# Semiconductor Device Physics for TFTs

Embed Size (px)

### Transcript of Semiconductor Device Physics for TFTs

Chapter 2Semiconductor Device Physics for TFTs

Abstract Two device physics topics are discussed in this chapter, namely, surfaceband bending and surface charges in the metalinsulatorsemiconductor, MIS,structure, and electron-hole pair recombination/generation processes. The treat-ment of the MIS structure covers the relationship between the voltage on the metalgate, the induced surface charge in the semiconductor and the resulting surfacepotential. This is treated analytically, using single crystal equations, and therelationships are fundamental to the understanding of IGFET operation. Equally,the concepts are widely employed in analysing TFT behaviour. The electron-holepair generation process underlies the leakage current behaviour of many semi-conductor devices, and can be applied to the analysis of TFT off-state behaviour.The recombination process determines steady state carrier concentrations underinjection conditions, such as optical illumination. Finally, there is a brief discus-sion of carrier flow in semiconductor devices, including the equations used innumerical simulation packages.

2.1 Introduction

In this chapter, device physics topics are introduced, which are relevant to TFTs,and for following the discussion in later chapters. The emphasis is on backgroundunderstanding of basic device physics principles, and an analytical approach isfollowed, using single crystal semiconductor equations. These concepts andequations are modified in later chapters for the more complex situation of the non-single crystal TFT materials.

The first topic presented deals with semiconductor surface physics, focussing onband bending and surface charge in the metalinsulatorsemiconductor, MIS,system. This underlies the relationship between the voltage on the metal gate andthe induced charge in the semiconductor surface, and introduces the concepts ofthe flat band voltage and the threshold voltage for surface inversion. The mostwidely studied semiconductor/insulator interface is the c-Si/SiO2 interface, and thenumerical examples given are based upon this system, although the equations

S. D. Brotherton, Introduction to Thin Film Transistors,DOI: 10.1007/978-3-319-00002-2_2, Springer International Publishing Switzerland 2013

9

themselves are quite general. In Chap. 6, these surface space charge equations arere-formulated to include the U-shaped density of states functions found in a-Si:Hand other TFT materials, and the influence of these extra states is compared to thesimpler situation discussed in this chapter.

The second topic is electron-hole pair generation and recombination. These arebasic processes underlying both leakage current effects, and steady state carrierdensities in devices under injection conditions, such as optical illumination.Finally, there is a brief discussion of carrier flow and the coupled field/spacecharge equations, which need to be solved in order to calculate the currentvoltagecharacteristics of a device.

Much current research into device behaviour makes use of commercial devicesimulators to solve these latter equations. These simulation packages give a deeperinsight into device behaviour by relating its currentvoltage characteristics tointernal field and carrier distributions. However, in published work, the funda-mental equations are rarely listed. In the final Sect. 2.4, of this chapter, thoseequations are presented, and they are built up from the material in the precedingsections of the chapter (but, the numerical techniques used for the solution of theequations go beyond the scope of this book).

As is apparent, the range of device physics topics covered here is limited, and,for a broader coverage of this field, there are many excellent books available, suchas Sze and Ng [1]. Examples of device simulation packages can be found in Refs.[2, 3], as well as a discussion of the numerical solution techniques in [2].

Some of the key simplified equations, from Sects. 2.2 and 2.3, are listed in theAppendix. These are useful for cross-reference purposes in later chapters, and alsofor direct, analytical calculations.

2.2 Semiconductor Surface Physics

2.2.1 Ideal MIS Capacitor and Surface Band Bending

Figure 2.1a shows the band diagram of an ideal MIS capacitor, on a p-type sub-strate, in which the Fermi levels in the metal and in the semiconductor perfectlyalign, such that there is no induced band bending within the structure (In Sect.2.2.3, a more realistic situation will be discussed, in which there are work functiondifferences between the metal and the semiconductor, and the semiconductorinterface contains interface trapping states). In the treatment below, the followingconventions will be used: the Fermi potential, VF, will be measured from the bulkintrinsic level, Ei, and will be taken as positive beneath Ei and negative above it.Similarly, the band bending, Vs, will be measured from the bulk intrinsic level, andthe polarity convention will be the same as used for VF.

When a positive charge, QG, is placed on the metal gate, it will induce an equaland opposite negative charge in the semiconductor, Qs, and this negative charge

10 2 Semiconductor Device Physics for TFTs

http://dx.doi.org/10.1007/978-3-319-00002-2_6

will consist of an increase in the electron density and a decrease in the free holedensity, thereby, leaving behind immobile, ionised acceptor centres, Na. In order toaccommodate these changes in free carrier density, the bands within the semi-conductor will have to bend downwards near its surface, as shown in Fig. 2.1b. Itwill also be seen that the positive charge on the gate results from a positive biasbeing applied to the gate relative to the semiconductor. Following the conventiondiscussed above, the Fermi level in the metal is moved downwards in response tothe positive gate bias, VG, and the semiconductor surface potential is +Vs. Thesituation shown in this diagram is for a small positive potential on the gate, suchthat the surface electron density, ns, is small compared with Na, and the surface issaid to be depleted (of free holes). For a larger positive gate bias, the situationshown in Fig. 2.1c occurs. In this case, there is a corresponding increase in bandbending, Vs, and the free electron concentration at the surface is larger than Na: thesurface is now said to be inverted. Between these two situations, when the bandbending, Vs = VF, the surface will be intrinsic, and ns = ps = ni. Further positive

Fig. 2.1 Ideal metalinsulatorsemiconductor, MIS, band diagrams, showing different surfacecharge conditions for a p-type substrate: a flat bands, b hole depletion, c electron inversion, andd hole accumulation

2.2 Semiconductor Surface Physics 11

band bending beyond this point will lead to ns [ ps. Finally, as shown in Fig. 2.1d,with a negative bias applied to the gate, there is an increase in positive chargeinduced in the semiconductor, due to an increase in the free hole density. This isassociated with the bands bending upwards by an amount -Vs. In this case, thesurface is said to be accumulated. With an n-type substrate, the opposite situationoccurs, in that a negative gate bias will cause the surface to be depleted/invertedrather than accumulated, and a positive bias will cause surface accumulation.

To establish the relationship between Vs, and Qs and VG, it is necessary to solvePoissons equation, where:

d2V

dx2 qqx

e0es2:1

e0 is the permittivity of free space, es is the dielectric constant of the semicon-ductor, and the space charge density, q(x) is:

qx px nx Na 2:2

The free carrier densities are defined by the intrinsic carrier concentration, ni,and the separation of the Fermi level from the intrinsic level, i.e.:

px ni expq VF V

kT

nx ni expq VF V

kT

2:3

px nx 2nishqVF V=kT 2:4

Where T is the temperature, and k is Boltzmanns constant. At the surface,V = Vs, and in the bulk, where V = 0:

p0 ni expqVFkT

and n0 ni expqVF

kT

From charge neutrality,1

p0 n0 Na 2nishqVF=kT 2:5

d2V

dx2 2niq

e0essh

qVF VkT

sh qVFkT

2:6

Using d2V

dx2 12 ddV dVdx 2

, and integrating Eq. 2.6 from the bulk (V = 0, anddV/dx = 0) to the surface (V = Vs, and dV/dx = -Fs):

1 VF = (kT/q)ln(Na/ni).

12 2 Semiconductor Device Physics for TFTs

dV

dx

2VVs F2s

4niqe0es

kT

qch

qVF VskT

kTq

chqVFkT Vssh

qVFkT

2:7

From Gauss Law, the surface field, Fs, is related to the total areal charge, Qs,contained within the surface by:

Qs e0esFs 2:8

Hence, the relationship between Qs and Vs is given by:

Qs ffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffi4niqe0es

pGVs;VF 2:9

where G(Vs, VF) is given by:

GVs;VF

ffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffikT

qch

qVF VskT

kTq

chqVFkT Vssh

qVFkT

s2:10

Given the positive and negative values of Qs in Eq. 2.9, the appropriate signs ofVs, Fs and Qs are given in Table 2.1, and the correct value of Qs is given by:

Qs VsVsj j

Qsj j 2:11

Equation 2.9 has been evaluated for a crystalline Si substrate doped with 1015

acceptors/cm3, and the key features in the relationship between Qs and Vs areshown in Fig. 2.2.2 The three previously discussed regimes of accumulation,depletion and inversion are indicated, and, for accumulation and inversion, Qsincreases exponentially with Vs. In these two regimes, the main contributors to Qsare the free carriers, so that the hole and electron densities increase exponentiallywith Vs in accumulation and inversion, respectively. In the third regime ofmajority carrier depletion, Qs increases with HVs, and extrapolating the inversionarm of the curve back into this regime shows that the ionised acceptor chargedominates Qs. Hence, in the three regimes, either free carriers or fixed spacecharge constitutes the major part of Qs. As will be seen in Chap. 6, this is notnecessarily the case with TFT materials, in which trapping states in the forbidden

Table 2.1 Polarity relationship between band bending, surface field and space charge in an MISstructure

Vs Fs Qs Free carrier conditions

+ve +ve -ve Reduction of holes and/or increase of electrons-ve -ve +ve Reduction of electrons and/or increase of holes

2 Note that in evaluating Eq. 2.10, if the units of Boltzmanns constant, k, are in eV/K, then q hasthe value of unity. If SI units are used, then q has its usual value of 1.602 9 10-19 C.

2.2 Semiconductor Surface Physics 13

http://dx.doi.org/10.1007/978-3-319-00002-2_6

band gap can continue to make a major contribution to Qs even when the surfacehas enough free carriers to support substantial conduction.

For the calculation in Fig. 2.2, the value of qVF was 0.288 eV below Ei, and theelectron concentration in inversion starts to dominate Qs at Vs [*2VF. In fact,the conventional definition of the threshold for strong surface inversion is atVs = 2VF, where the volume concentration of free electrons at the surface, ns, isequal to the volume concentration of acceptors, Na. When Vs = VF, the surface isintrinsic (ns = ps = ni), and the band bending regime beyond this, and up to stronginversion, is referred to as weak inversion (ps \ ns \ Na).

In the depletion/inversion regime, the band bending, Vs, is positive, and for Vs,and VF [ kT/q, i.e., more than kT from the flat band position, Eq. 2.9 can besimplified to:

Qs ffi ffiffiffiffiffiffiffiffiffiffiffiffi2qe0es

pni

kT

qexp

qVs VFkT

NaVs 0:5

2:12

The first term in the brackets relates to the free electron concentration, and thesecond term to the ionised acceptor space charge density, and the dependence ofthose terms on Vs shows the exponential and quadratic forms, respectively, dis-cussed above. This simplified expression, with the physically obvious terms,provides a good approximation to the full Eq. 2.9, as seen by the calculations inFig. 2.3. The calculations used two different substrate doping levels, and, for themore heavily doped substrate, with 1016 acceptors/cm3, the value of qVF is0.348 eV below Ei, and this correspondingly increases the value of Vs at whichstrong inversion occurs. Also, the increase in Qs, for the more heavily dopedsubstrate, at a given value of Vs in depletion, is *3 times more than for the lessheavily doped substrate, as expected from the HNa dependence in Eq. 2.12.

Between flat bands and inversion, when the ionised acceptor space chargedominates, Eq. 2.12 can be further reduced to:

Fig. 2.2 Calculated variationof surface charge density withsurface potential (substratedoping density is1 9 1015 acceptors/cm3)

14 2 Semiconductor Device Physics for TFTs

Qs ffi ffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffi2qe0esNaVs

p Qb 2:13

Where Qb is the areal acceptor space charge density. Equation 2.13 is the sameas directly calculated from Poissons equation using the depletion approximation,i.e. from:

d2V

dx2 qNa

e0es2:14

and integrating this with respect to V. Alternatively, if Eq. 2.14 is integrated withrespect to x, then:

Qs qNaxd 2:15

where xd is the width of the space charge depletion region at Vs. At inversion,when Vs = 2VF, further increases in band bending cause such large increases inQs, due to the exponentially increasing free electron density, that, to a firstapproximation, the fixed space charge can be regarded as having reached a limitingmaximum value, Qbmax. This can be obtained by substituting Vs = 2VF intoEq. 2.13:

Qbmax ffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffi2qe0esNa2VF

p2:16

and from Eq. 2.15,

Qbmax qNaxdmax 2:17

where xdmax is the maximum width of the depletion region, and, from Eqs. 2.16and 2.17, xdmax is given by:

xdmax ffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffi2e0es2VF

qNa

s2:18

Fig. 2.3 Comparison ofsurface charge densitycalculations using the full(solid line) and approximate(symbols) expressions fromEqs. 2.9 and 2.12,respectively. (Substratedoping densities of 1 9 1015

acceptors/cm3, and 1 9 1016

acceptors/cm3)

2.2 Semiconductor Surface Physics 15

Qs in Eq. 2.12 can be represented by the sum:

Qs Qn Qb 2:19

Where Qb is the extended depletion layer charge, and Qn is the areal density ofinversion layer electrons. These will be confined close to the semiconductor sur-face, by virtue of the electrons being in a parabolic potential well of depth Vs. Theterms in Eq. 2.19 are pictorially represented in Fig. 2.4a for inversion (Vs [ 2VF),and by Fig. 2.4b for depletion (Vs \ 2VF). The variation of xdmax with Na can becalculated from Eq. 2.18, and is shown in Fig. 2.5. From a TFT point of view,assuming a certain equivalence between Na and the TFT trap state density, a curveof this type can be used to determine whether a thin film is fully depleted or not atinversion. For instance, the maximum equilibrium space charge width, at inver-sion, for a substrate doped with 1017 acceptors/cm3 is 100 nm; therefore, a thinfilm of 100 nm, with an equivalent volume trapped charge density of\1017 cm-3,will be fully depleted before Vs = 2VF. As a result of this, the threshold ofinversion will occur at a lower value of band bending than for a thicker film havingthe same trap state density. This is discussed further in Chap. 3

Fig. 2.4 Illustration of bulk depletion layer, Qb, and inversion layer, Qn, charge densities in:a inversion, and b depletion

Fig. 2.5 Variation ofmaximum depletion layerwidth at inversion, xdmax,with substrate doping level

16 2 Semiconductor Device Physics for TFTs

http://dx.doi.org/10.1007/978-3-319-00002-2_3

2.2.2 Gate Bias and Threshold Voltage

Referring to Fig. 2.1, the voltage on the gate, VG, is dropped partially across thedielectric, Vi, and partially across the semiconductor, Vs, so that:

VG Vi Vs 2:20

And, for charge neutrality, the charge on the gate, QG, equals the charge in thesemiconductor, Qs, and

QG e0eiFi e0eiVi=di CiVi Qs 2:21

Where Fi is the field in the gate dielectric, and Ci is the capacitance/unit area ofthe gate dielectric. Hence,

VG Vs Qs=Ci 2:22

Equation 2.22 can be used to relate the voltage on the gate of an MIS capacitorto the induced charge density in the semiconductor, Qs, and to the associated bandbending, Vs. It can also be used to calculate the threshold voltage, VT, of thestructure, i.e. the gate voltage necessary to induce band bending of 2VF at thesemiconductor surface:

VT 2VF ffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffi2qe0esNa2VFp

Ci2:23

Figure 2.6 shows the calculated variation of VG with Vs for the two substratedoping levels used in Fig. 2.3, and for a 150 nm thick gate dielectric of SiO2. Themore heavily doped substrate requires a larger gate bias to achieve a given degreeof band bending in depletion, and, equally, has a larger value of VT, as shown byEq. 2.23. Once the surface has gone into strong inversion, the free electron den-sity, Qn, dominates Qs, and Qn is given by:

Qn Ci VG VT 2:24

As will be seen in Chap. 3, this is a widely used expression for the calculationof channel currents in MOSFET devices above threshold. It is equally widely usedfor similar calculations in TFTs. Hence, the threshold voltage is a key parameter indetermining on-state device characteristics, and the dependence of thresholdvoltage on substrate doping level is shown in Fig. 2.7.

2.2.3 Real MIS Structures

In contrast to the idealised MIS structure shown in Fig. 2.1, real structures mayhave work function differences between the gate metal and the semiconductor,

2.2 Semiconductor Surface Physics 17

http://dx.doi.org/10.1007/978-3-319-00002-2_3

fixed charges in the oxide, and interface trapping states at the dielectric/semi-conductor interface. These will change the zero-gate-bias band bending, and affectthe relationship between VG and Vs and Qs.

2.2.3.1 Work Function Differences

In general, the Fermi level position in a free metal will be different from the Fermilevel in a free semiconductor. These differences are usually expressed in terms of awork function difference, where the work function is the energy required to remove

Fig. 2.7 Calculated variationof threshold voltage withsubstrate doping level, andthickness of SiO2 gatedielectric

Fig. 2.6 Calculated variation of surface potential, Vs, with gate bias, VG, in an ideal MISstructure, and showing the threshold voltage points. (Dielectric layer of 150 nm of SiO2, and p-type substrate doping of 1 9 1015 cm-3, and 1 9 1016 cm-3)

18 2 Semiconductor Device Physics for TFTs

an electron from the Fermi level to the vacuum level. When the two materials areconnected, and in thermal equilibrium, the Fermi levels need to be coincident, andthere will be a flow of electrons from one material to the other, resulting in aninterfacial dipole, which establishes this equilibrium. In the semiconductor, this willresult in surface band bending, the extent of which will be much greater than in themetal due to the short screening length of the latters high electron density.

In an MIS structure, it is conventional to reference the Fermi levels to thedielectrics conduction band edge [4] (rather than to the vacuum level), so that thequoted barriers, UMi and vi, are the energies needed to remove an electron to thedielectric conduction band (as shown in Fig. 2.8, and v is the electro-negativity ofthe semiconductor). For the Si/SiO2 system, these barrier energies were experi-mentally established by photo-emission measurements from the metal gate or thesemiconductor into the oxide conduction band, and were 0.51 eV less than therespective vacuum values [5]. Figure 2.8a schematically shows the metal and thesemiconductor separated, and Fig. 2.8b shows them connected in thermal equi-librium. In this case, electrons have flowed from the metal to the semiconductor tobring the Fermi levels into coincidence. As a result of this, the bands in thesemiconductor have bent downwards by Vs0, with a corresponding voltage dropacross the dielectric of Vi0. Equating the potentials either side of the high point inthe insulator conduction band:

UMi Vi0 vi Ei=q VF Vs0 2:25

The metalsemiconductor work function difference, UMS, is, therefore, given by:

UMS UMi vi Ei=q VF Vi0 Vs0 2:26

Thus, to remove the zero gate bias band bending in the system, and to restoreflat band conditions, the gate voltage needs to be made more negative to induce

Fig. 2.8 MIS energy band diagrams in the presence of metalsemiconductor work functiondifferences: a separated metalinsulator and insulatorsemiconductor, b MIS system in thermalequilibrium

2.2 Semiconductor Surface Physics 19

more positive charge in the semiconductor surface. The gate voltage at flat bands,VFB, is given by:

VFB UMS Vi0 Vs0 ffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffi2qe0esNaVs0p

Ci Vs0

2:27

Equally, the gate voltage required to achieve a given degree of band bending,including the threshold for inversion, will be modified by the metalsemiconductorwork function difference, so that the expression for the threshold voltage nowbecomes:

VT VFB ffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffi2qe0esNa2VFp

Ci 2VF 2:28

As indicated in Eq. 2.26, the work function difference will be a function both ofthe gate metal, and of the doping level in the semiconductor substrate, as shown inFig. 2.9 for Al and doped poly-Si gates [1]. Due to its refractory properties, dopedpoly-Si has been extensively employed as the gate electrode in MOSFET tech-nology, and, with appropriate doping, it can be tailored to produce the requiredsign of flat band voltage.

2.2.3.2 Oxide Charges and Interface States

Many gate dielectrics, including SiO2, are characterised by charged centres in theoxide, which induce an opposite charge in the semiconductor surface. If thecharged centres, Qi, are located at a distance x from the dielectric-semiconductorinterface in an MIS capacitor, the charge induced in the semiconductor, Qs, is:

Qs Qi d x =d 2:29

Fig. 2.9 Experimentallydetermined MOS work-function differences, UMS, asa function of Si-substratedoping level, for differentgate contact materials.(Reproduced from [1] withpermission of John Wiley &Sons, Inc)

20 2 Semiconductor Device Physics for TFTs

Hence, for charges at the dielectric/semiconductor interface, the induced chargeis equal to the charge, Qi, in the dielectric, whilst those at the metal interface haveno effect. In many cases, the location of the charges may not be known, and aneffective charge density, Qieff, will be determined, as though it were located at thedielectric/semiconductor interface.

As with the work function difference, this will result in a non-zero flat bandvoltage, given by:

VFB Qieff=Ci 2:30

Positive charges are commonly found in SiO2 films on Si, and are referred to asfixed charges, as their effect is not dependent upon the surface potential in thesemiconductor. In other words, they have a constant effect, irrespective of the biasconditions, and present a fixed density.

In real crystalline semiconductor surfaces, the termination of the regular,periodic bulk potential introduces allowed states into the forbidden band gap,usually referred to as surface states. These are intrinsic states at the surface, and, inaddition to these, there may be extrinsic states due to impurities. The densities ofintrinsic states can be up to *1015 cm-2 on an atomically clean surface, but, in awell-passivated surface, such as the Si/SiO2 interface produced by thermal oxi-dation of Si, these can be reduced to \15 9 1012 cm-2. The reduction is due tothe SiO2 network providing oxygen pairing atoms for the Si dangling bonds, andfurther passivation with hydrogen typically reduces the overall density to*1010 cm-2 or less. This combination of thermal oxidation and hydrogen pas-sivation has generated one of the best-controlled semiconductor interfaces, andprovided the basis for the Si semiconductor device industry.

Surface or interface states are generally distributed in energy across the for-bidden band gap, and, in the case of the Si/SiO2 interface, the distribution isU-shaped between the valence and conduction band edges. In contrast to the fixedcharge, the charge in interface states will be determined both by their distributionacross the band gap, and by the position of the Fermi level at the surface. Using thezero Kelvin approximation, those states beneath the Fermi level can be regarded asfilled with electrons, whilst those above will be empty. Take, for example, aconstant density, Nss(E), across the band gap, with acceptor levels in the upper halfof the band gap, and donor levels in the lower half, and with a neutral level, E0, atmid-gap. This distribution will have zero net charge in the interface states whenthe surface Fermi level is at mid-gap. However, if this distribution were added tothe MIS band diagram used in Fig. 2.1a, where the Fermi level is below mid-gap,there would be a flow of electrons from the interface states below E0, leading topositively charged, empty donor states at the surface, and an equal negative chargedensity in the semiconductor surface. Hence, the semiconductor bands at thesurface will be bent down by an amount Vs0 to ensure charge neutrality betweenthe interface and the bulk, as shown in Fig. 2.10. In this example, the block ofdonor states between EF and E0 would be empty of electrons, and have a positivecharge, Qss, balanced by the negative semiconductor surface charge, Qs.

2.2 Semiconductor Surface Physics 21

In general, the electron occupancy, F(E), of a surface state at energy E is givenby the FermiDirac distribution function:

FE 11 expqVF qVS E=kT

2:31

Using the polarity convention of the earlier sections, E will have a negativevalue for centres above E0 (which is at mid-gap), and a positive value for thosebelow. Hence, the total negative charge in the surface states, Qss

-, with bandbending Vs [ VF is:

QssVs ZECE0

qNssEFEdE ZE0qVsVF

E0

qNssEdE 2:32

In Eq. 2.32, the full integral expression, which includes the FermiDiracfunction, can be reduced to the simpler analytical form by using the zero Kelvinapproximation, in which the acceptor states are negatively charged between theneutral level and the surface Fermi level, and neutral above the Fermi level. For auniform distribution of acceptor states, Nss can be brought outside the integral, andthe density of negatively charged states, when Vs [ VF, is:

QssA qNssqVs VF 2:33

Similarly, for Vs \ VF (as shown in Fig. 2.10), the density of positivelycharged donor states is:

Fig. 2.10 Zero gate-biasMIS band diagram with auniform distribution ofinterface states across theband gap, and with the cross-hatched region showing thecharged states. (Donor andacceptor states in the lowerand upper halves of the band-gap, respectively, and withthe neutral level at mid-gap)

22 2 Semiconductor Device Physics for TFTs

QssD qNssqVF Vs 2:34

For a constant distribution of surface states, the zero Kelvin approximation is auseful simplification. However, for trapping state distributions where the densityvaries significantly over an energy interval of kT, it is less accurate, and anumerical evaluation of the full integral in Eq. 2.32 would be required. This issueis discussed further in Sect. 6.2.3, where the volume trap density in a-Si:H variesexponentially with position from the band edge.

As with the work function difference and the fixed oxide charge, a bias, VFB,will need to be applied to the gate to establish the flat band condition in thesemiconductor, where VFB is given by:

VFB QssDVs 0

Ci qNssqVF

Ci2:35

However, in contrast to the fixed oxide charge, the presence of interface stateswill give more than just a constant shift in the relationship between VG and Vs andQs. In particular, as Vs is increased, not only does the gate bias need to induce theincreasing value of Qs, but it must also supply the increasing charge going into theinterface states. The relationship between VG and Vs from Eq. 2.22 is modified tobe:

VG Vs QsCi Q

ssDCi

QssACi

2:36

and, for the example being used, Qss(A) = 0 for Vs \ VF, and Qss(D) = 0 forVs [ VF, and the non-zero values of Qss(A) and Qss(D) are negative and positive,respectively.

Figure 2.11a compares the relationship, between VG and Vs, for an ideal trap-free interface (Nss = 0) and an interface containing a range of Nss densities from1 9 1010 cm-2 eV-1 to 1 9 1013 cm-2 eV-1. The lowest interface state densityof 1010 cm-2 eV-1 is so low that the VGVs relationship is indistinguishable fromthe trap-free case. However, for the higher densities, increasingly large values ofVG are required to achieve a given amount of band-bending due to the chargegoing into the interface states. The curves have a common crossing point atVs = 0.288 V, when the surface Fermi level is at mid-gap. This corresponds to theneutral level of the interface states, so that all the interface state distributions havethe same zero charge in them. The flat band voltages can also be directly read fromthe curves by the values of VG corresponding to Vs = 0 V.

The other parameter which can be extracted from these curves is the value of Vswhen VG = 0, which is the equilibrium zero-gate-bias bend banding, Vs0, and thesevalues, together with the corresponding values of Qss (at Vs0), are shown inFig. 2.11b. The S-shaped curves demonstrate some simple physical principles ofcharge trapping over the range of Nss values used. For low Nss values, such as1010 cm-2 eV-1, the Fermi level position at the surface is dominated by the sub-strate doping level, and the surface states have almost no effect. In this case, the Nss-

2.2 Semiconductor Surface Physics 23

http://dx.doi.org/10.1007/978-3-319-00002-2_6

induced band bending tends towards zero, and the interface states are ionised almostdown to the position of the bulk Fermi level, and Qss * qNssqVF. Although asubstantial fraction of the states are ionised, the charge in them is so low, thatnegligible band bending is required to produce an approximately equal amount ofcharge in the substrate. In contrast, for high Nss values, such as 10

13 cm-2 eV-1, theband-bending is dominated by the charge in the surface states, and the Fermi leveltends towards being pinned at the surface state neutral level, i.e. Vs0 ) VF. In thiscase, VF-Vs0 = 0.01 V, and the surface state neutral level is just 100 meV abovethe Fermi level. However, with the large surface state density, this still correspondsto a substantial charge, Qss, in the fractionally ionised donor surface states. Forintermediate values of Nss between 10

11 and 1012 cm-2 eV-1, there is a progressiveincrease in Vs0 with Nss, and Qss is given by qNssq(VF-Vs0).

Equation 2.36 also shows that the charge going into surface states has to beallowed for in calculating the gate threshold voltage for surface inversion. Thesurface potential at which this occurs is still 2VF, but the gate bias, in excess of theflat band voltage, to achieve this surface potential is increased to:

VT VFB ffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffi2qe0esNa2VFp

Ci 2VF

QssVs 2VFCi

2:37

and, as Qss(D) = 0 for Vs [ VF, only charge in the acceptor states will contribute,and from Eq. 2.33, Qss(A) at inversion is given by:

QssA qNssq2VF VF qNssqVF 2:38a

Finally, the effects of the work function difference, the dielectric charge and thecharge in interface states are all independent and additive, so that, in the presenceof all three, the flat band voltage is given by:

Fig. 2.11 Calculations using the uniform interface state distribution shown in Fig. 2.10a variation of gate bias with surface potential, Vs, for different values of Nss, and b variationof zero gate bias band bending, Vs0, and Qss (at Vs0) with Nss. (Substrate acceptor density,Na = 10

15 cm-3, qVF = 0.288 eV, tox = 150 nm, and interface state density, Nss = 1010

1013 cm-2 eV-1)

24 2 Semiconductor Device Physics for TFTs

VFB UMS Qieff=Ci Qss Vs 0 =Ci 2:38b

2.2.4 Evaluation of Surface Potential

From Eq. 2.9, the surface potential, Vs, uniquely defines the space charge density,Qs, and Eqs. 2.22 and 2.36 define the gate bias, VG, needed to achieve that potential,with and without surface states, respectively. Therefore, the measurement of Vsfacilitates a quantitative insight into the state of a semiconductor surface. A commontechnique for establishing Vs is through the small signal capacitance-voltage mea-surement of an MIS diode, where the capacitance is given by:

C dQGdVG

dQsdVG dVs

dVG

dQsdVs

dVGdVs 1 1

Ci

dQsdVs

anddQsdVs Cs

)C 1= 1=Ci 1=Cs

2:39

In other words, the capacitance of the MIS diode is the series combination ofthe capacitance of the dielectric, Ci, and of the semiconductor surface, Cs, whereCs is given by the differentiation of Eq. 2.9:

Cs ffiffiffiffiffiffiffiffiffiffiffiffiffiffiniqe0esp

shqVs VF=kT shqVF=kT GVs;VF

2:40

and G(Vs, VF) is given by Eq. 2.10. The normalised CV curves resulting from theevaluation of Eq. 2.40, for a silicon substrate doped with 1015 and 1016 acceptors/cm3, and a gate oxide thickness of 150 nm, are shown by the solid lines in

Fig. 2.12 Normalised highand low frequency MIS CVcurves (calculated for 150 nmthick SiO2 gate dielectric)

2.2 Semiconductor Surface Physics 25

Fig. 2.12. These curves have a characteristic V shape, with the capacitance atnegative VG values tending towards the capacitance of the gate dielectric, due tothe large capacitance of the hole accumulation layer. With increasing positive VG,the capacitance falls due to the growth of the hole depletion region at the surface,which progressively reduces the surface capacitance. Finally, the curves start torise as the surface becomes strongly inverted, and the large free electron con-centration screens the underlying depletion layer, with the total capacitance onceagain tending towards the value of the gate dielectric.

As these curves have been calculated for an ideal MIS diode, the energy bandswill be flat at VG = 0, and, hence, the normalised capacitance at flat bands can bedirectly obtained from the curves. Given the unique relationship between surfacepotential and capacitance, the flat band voltage can, in principle, be directlyobtained from any experimental CV measurement using Eq. 2.40, assuming thatthe substrate doping level is known. Moreover, the minimum capacitance is also aunique function of doping level and dielectric capacitance, so that the doping levelcan be extracted from the minimum of the experimental CV curve. The nor-malised flat band and minimum capacitance values from Fig. 2.12 are listed inTable 2.2, and they have also been extensively tabulated by Sze and Ng [1]. Alsomarked on the curves in Fig. 2.12 are the capacitance values at which the bandbending gives an intrinsic surface (Vs = VF), and the threshold for an invertedsurface (Vs = 2VF).

The solid line calculations assume thermal equilibrium, and the increase incapacitance in inversion will only be observed experimentally if the free electronsin the inversion layer can follow the a.c. measuring signal. In a high quality Si/SiO2 capacitor, the inversion layer response time can be of the order of seconds, ormore [6], as it depends upon a thermal generation process within the surface spacecharge region. Hence, the calculated curves are only likely to be replicated with alow frequency measurement, and the solid line curves in Fig. 2.12 are oftenreferred to as low frequency CV curves. Moreover, in the presence of interfacestates, there can be a further complication in the interpretation of the experimentallow frequency curves. This will arise if the occupancy of the interface states at theFermi level can follow the measuring signal, and, hence, contribute an interfacestate capacitance, Css, in parallel with the semiconductor surface capacitance Cs.The surface state capacitance, Css, is given by:

Css dQssdVs qNss 2:41

Table 2.2 Relationship between normalised flat band capacitance, minimum CV capacitanceand substrate doping level (for 150 nm SiO2 gate dielectric)

Na (cm-3) CFB/Ci Cmin(LF)/Ci Cmin(HF)/Ci

1 9 1015 0.77 0.38 0.321 9 1016 0.91 0.63 0.59

26 2 Semiconductor Device Physics for TFTs

where, as discussed in the previous section, Qss can be approximated byqNssq(Vs-VF) for constant (or slowly varying) surface state densities. The pres-ence of Css in an experimental CV measurement means that Eq. 2.40 can nolonger be used to give a unique relationship between measured capacitance andband bending, Vs. By implication, a high frequency measurement can be used tominimise the capacitive contributions of the surface states, and will also suppressthe free electron capacitance in strong inversion. Hence, to interpret the highfrequency CV curves, a high frequency version of Eq. 2.40 is required. Thisessentially means suppressing the electron response in inversion, and this can beaccomplished by expanding the cosh and sinh terms containing Vs, and setting tozero those of the form expq(Vs-VF)/kT, since, in inversion, Vs [ VF and thoseterms will govern the electron contribution to the surface capacitance. Hence thehigh frequency expression, Cs(HF) is given by:

Cs ffiffiffiffiffiffiffiffiffiffiffiffiffiffiniqe0esp 0:5 expqVs VF=kT shqVF=kT

G0Vs;VF2:42

and G0(Vs,VF) is given by:

G0Vs;VF

ffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffi0:5

kT

qexp

qVF VskT

kTq

chqVFkT Vssh

qVF

kT

s2:43

The high frequency CV curve, calculated from Eq. 2.42, for qVs [ 3kT, isshown by the dotted lines in Fig. 2.12. The inversion layer response has beensuppressed, and the surface capacitance in inversion tends to a constant value,approximately given by:

CsHF e0es

xdmax2:44

Where xd(max) is the limiting maximum thickness of the surface depletionregion, as discussed in Sect. 2.2.1, and is given by Eq. 2.18. As with the minimumcapacitance value of the low frequency curves, the minimum value of the highfrequency curves is also a unique function of doping level, and can be used toestablish the doping level in experimental samples. These values are also shown inTable 2.2. More importantly, any horizontal displacement, DVG, of an experi-mental CV curve from the theoretical CV curve can be used to establish Qss, as afunction of Vs, from:

Qss Vs DVG=Ci 2:45

and Nss can then be derived from dQss/dVs.Whilst the emphasis in this section has been on high frequency measurements,

and the use of the measured MISC capacitance to establish surface potential, thereis also a low frequency procedure, called the quasi-static CV measurement, whichuses the change in capacitance, at a given value of VG, to determine Nss [7, 8].Finally, to complete this section, one other well-established technique for the

2.2 Semiconductor Surface Physics 27

evaluation of surface state densities should be mentioned, and this is the a.cconductance measurement of MISCs [9]. A detailed overview of these procedurescan be found in Sze and Ng [1].

2.3 Electron-Hole Pair Generation and Recombination

Electron-hole pair generation and recombination are fundamental semiconductorprocesses relevant to both off-state leakage currents and to steady-state photo-currents in TFTs.

Two sources of leakage current in semiconductor devices are by ohmic con-duction in lightly conducting and/or low generation lifetime material, or byelectron-hole pair generation and/or diffusion current flow in reverse biasedjunctions. The latter processes are illustrated in Fig. 2.13a for a reverse biased n+pjunction. Due to the field within the space charge region, the holes generatedwithin this region are swept into the p-type substrate, where they constitute anohmic (drift) hole current to the substrate contact, Idrift. Equally, the electronsgenerated in the space charge layer are swept into the n+ region, where they flow tothe n+ contact. For current continuity, there will be equal hole and electron cur-rents, and these are referred to as generation currents. The electron-hole pairgeneration process, from a deep lying centre within the forbidden band gap, isshown schematically in Fig. 2.13b. In addition to the direct generation process,there is also a diffusion current, Idiffn, of minority carrier electrons from the neutralp-type substrate into the adjacent depletion region.

The role of electron-hole pair generation on leakage currents, including thediffusion current, is discussed in Sect. 2.3.3, and the recombination processes arepresented in Sect. 2.3.4.

Fig. 2.13 Illustration of a reverse biased n+-p junction, showing generation and diffusionleakage currents, and b eh pair thermal generation process

28 2 Semiconductor Device Physics for TFTs

In order to develop the expressions for electron-hole pair generation andrecombination, it is necessary to consider the basic processes of carrier emissionand carrier capture by a deep level centre, based upon the Shockley, Read, Hall(SRH) recombination statistics [10, 11], and the extension of this analysis to pnjunction characteristics [12].

The term deep level centre refers to intrinsic or extrinsic defects having energylevels within the forbidden band gap of the semiconductor, and which are usuallyfurther from the band edges than the shallow level dopant impurities. A deep levelcentre can behave as a trap, or as a generation centre, or as a recombination centre,depending upon its environment. For instance, in thermal equilibrium, a deep levelacceptor in n-type material can capture electrons, thereby, reducing the free carrierdensity, and is acting as trap.3 In a reverse biased space charge region, it can act asa generation centre, sequentially emitting electrons and holes, resulting in areverse bias leakage current. Or, in material subject to electron-hole pair injection,it can act as a recombination centre, where the sequential electron and hole captureprocess establishes the steady-state free carrier density under the injection con-ditions. Hence, all three terms are often used interchangeably to refer to the samedeep level centre, and, for brevity, the term trap is used as the generic term for thecentre in this section.

2.3.1 Thermal Equilibrium

For a deep level centre within the semiconductors forbidden band gap, four carriertransitions can be identified, as shown in Fig. 2.14. If the trap is an acceptor level, ithas two charge states, one of which is negatively charged when it is occupied by anelectron, and the other is neutral when it is empty of the electron (These two chargestates can be equivalently described in terms of hole occupancy, which are empty

Fig. 2.14 Carrier emission and capture processes from a deep level centre in the forbidden bandgap: a electron emission, b electron capture, c hole emission d hole capture. The horizontal blockarrow shows the states occupancy after the transition

3 The Fermi level position and the free electron concentration can be obtained from thenumerical solution of the charge neutrality equation: n NT Nd .

2.3 Electron-Hole Pair Generation and Recombination 29

and filled, respectively. The same transitions will occur from a deep donor centre,the only difference being that it is positively charged when empty of an electron andneutral when occupied by an electron). Hence, there is a pair of possible carriertransitions from each of the two charge states, as shown in Fig. 2.14. From thenegatively charged acceptor centre, these are either (a): electron emission to theconduction band, by a thermally stimulated process, or (d): hole capture from thevalence band, and the release of phonon energy back to the lattice. Both leave behindthe neutral centre. From the neutral centre, the two possible transitions are (b):electron capture from the conduction band, or (c): thermally stimulated hole emis-sion to the valence band (which is equivalent to electron emission from the valenceband). Both leave behind the negatively charged centre.

If the density of traps/generation/recombination centres is NT, and if the centreand the Fermi level are positioned at ET and EF, respectively, above the valence bandedge, then the trap occupancy is defined by the FermiDirac distribution function,and from this the carrier transition rates can be calculated. These rates are deter-mined by the number of free carriers and the appropriate occupancy of the centre, forthe capture process, or just by the occupancy of the centre for the emission process(where it is implicitly assumed that there are sufficient empty states in the bands toaccommodate the emitted carriers). In thermal equilibrium, the fractional electronoccupancy of the trap, FD(ET, EF), is given by the FermiDirac distribution function:

FD 1

1 expET EF=kT2:46

The free carrier densities, n0 and p0, in n-type material doped with Nd donors,are given by4:

n0 NT Nd NC expEC EF=kT ; p0 NV expEF=kT 2:47

and n0p0 n2i 2:48

The electron emission rate, Ree is:

Ree enNT enNT FD 2:49

where en is the electron emission rate constant. Similarly, the rate of hole emission,Rhe, is:

Rhe epN0T epNT1 FD 2:50

where ep is the hole emission rate constant. The rates of electron capture, Rec, andhole capture, Rhc, are:

Rec cnn0N0T rnvthn0NT1 FD 2:51

4 From 2.47, if NT Nd, EF kT lnNdNV=n2i .

30 2 Semiconductor Device Physics for TFTs

Rhc cpp0NT rpvthp0NT FD 2:52

where the electron and hole capture rate constants, cn and cp, are given by theproduct of the traps capture cross section, rn and rp, respectively, and the carriersthermal velocity, vth. The thermal velocity is H(3kT/qm*), where m* is theeffective mass, so that the thermal velocities for holes and electrons are differentfrom each other. However, for simplicity in this analysis, they are taken to be thesame.

In thermal equilibrium, the rate of electron capture must equal the rate ofelectron emission, and the equivalent equality must also exist for the hole tran-sitions. Hence,

enNT FD rnvthn0NT1 FD 2:53

And substituting for FD and n0, using Eqs. 2.46 and 2.47, respectively:

en rnvthNC expEC ET=kT 2:54

Similarly, for the hole transitions:

ep rpvthNV expET=kT 2:55

Hence, the thermal emission rate constants, en and ep, are fundamental prop-erties of the trap itself, and not dependent on the local concentrations of carriers.Moreover, their values are exponentially dependent upon the separation of the trapfrom the band edges.

2.3.2 Non-equilibrium, Steady State

Under steady state, non-thermal equilibrium conditions (where np 6 n2i ), the trapwill achieve a new occupancy, described by its quasi-Fermi level, and determined bythe equality of the net electron transition rate and the net hole transition rate,5 i.e.

dNTdt Rec Ree Rhe Rhc 0 2:56

In contrast to the thermal equilibrium situation, the rates of electron emissionand electron capture will not be equal. This is the situation in which there will be anet recombination or a net generation process, depending upon the divergence ofthe carrier concentrations from their thermal equilibrium values. Substituting therate constants into Eq. 2.56 gives:

ncnN0T enNT pcpNT epN0T 2:57

5 If these rates are not equal, then the trap occupancy will change with time.

2.3 Electron-Hole Pair Generation and Recombination 31

From Eq. 2.57, and using N0T NT NT , the hole occupancy is:

N0T NTen pcp

ncn pcp en ep2:58

This can be used to calculate the net local electron generation/recombinationrate, RGR, which, in steady state, will also be equal to the net hole recombination/generation rate, i.e.:

RGR Ree Rec NT en ncnN0T 2:59

Substituting for the trap occupancy terms:

RGR NTenep npcncp

ncn pcp en ep2:60

RGR rnrpvthNT fNC:NV expEC ET=kT : expET=kTg nprnn NC expEC ET=kT rpp NV expET=kT

2:61

Eliminating the exponential terms in ET in the numerator, and replacing theremaining exponential term by n2i ; gives the following expression:

RGR rnrpvthNT n2i np

rnn NC expEC ET=kT rpp NV expET=kT2:62

The numerator shows that the rate of recombination/generation is proportionalto the term n2i np, which expresses the deviation of the carrier population fromthermal equilibrium. For np [ ni

2, the free carrier excess stimulates a net recom-bination process, where the carrier excess could result, for example, from opticalillumination of the device, the forward biasing of a pn junction or avalanchegeneration at a reverse biased p-n junction. For np \ ni

2, the free carrier deficitgives rise to net generation, and the free carrier deficit is most commonlyencountered in the depletion region of a reverse biased pn junction. In thermalequilibrium, the net rates of recombination or generation are zero.

Equation 2.60 (or its equivalents 2.61 or 2.62) would be typically used indevice simulation packages to calculate the local rates of recombination or gen-eration, but, for analytical work, a simplified version of this expression is oftenused by making the simplifying assumption that rn = rp = r, and:

RGR rvthNT n2i np

n p 2nicoshET EikT2:63

where the following substitutions have been used for NC and NV in thedenominator:

ni NC expEC Ei=kT NV expEi=kT 2:64

32 2 Semiconductor Device Physics for TFTs

2.3.3 Generation Currents

As mentioned above, the general treatment of generation or recombination is fullyspecified by the use of Eq. 2.60, and, in this section, an approximate, but moreaccessible, analytical treatment is presented for describing generation currents. Forinstance, in the space charge layer of a reverse biased junction, as shown inFig. 2.13a, the free carrier concentrations can be taken as zero, so that there are nocarrier capture processes, and Eq. 2.60 reduces to an expression for the local,steady state generation rate, RG:

RG NT enepen ep

2:65

The steady state leakage current, JR, due electron-hole pair generation, in areverse biased p-n junction depletion layer of width W is:

JR qZW

0

RGdx qRGW qWNTenep

en ep2:66

Where it is assumed that RG is constant across W, and, in analogy withEq. 2.18, W is given by:

W

ffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffi2e0esVR V0

qNa

s2:67

VR is the reverse bias, and V0 is the built-in pn junction potential.Returning to Eq. 2.66, the ratio enep/(en ? ep) is a maximum when the

denominator is a minimum, which will occur when en = ep, and the traps are sitedclose to mid-gap. As ET moves away from mid-gap either en or ep will increaseexponentially, as will the sum en ? ep, whilst the product enep will be invariant.Hence, any centres located at mid-gap are likely to be the most efficient generationcentres, and will dominate the device leakage current, JR. For mid-gap centres,with equal capture cross sections, r:

en ep rvthNC expEi=kT rvthni 2:68

) JR qRGW 0:5qniWrvthNT 2:69

The generation lifetime, sg, is a figure of merit for the leakage current, and isdefined by the following relationship:

JR qniW=sg 2:70

Hence, for mid-gap centres, the generation lifetime is:

sg 1=0:5NTrvth 2:71a

2.3 Electron-Hole Pair Generation and Recombination 33

If the capture cross-sections are not equal:

sg 1=NTrnvth 1=NTrpvth 2:71b

Equation 2.71b explicitly shows that the rate of the two-stage generation pro-cess is determined by the sequential emission of holes and electrons, and, if onecapture cross-section is larger than the other, then the overall generation processwill be rate limited by carrier emission from the charge state of the centre havingthe smaller cross-section. In experimental samples, this difference in capture cross-sections is likely to be found. For example, if the trap is an acceptor, then it will beneutral before capturing an electron, and negatively charged before capturing ahole. The Coulombic attraction between the hole and the negatively charged centrewill result in the hole capture cross-section being larger than the neutral cross-section for electron capture [13]. As an example of this, one of the most widelystudied deep level centres in silicon is gold, which has a near mid-gap acceptorlevel at 0.54 eV below the conduction band edge, and its capture cross-sections are1.5 9 10-14 cm2 and 9 9 10-17 cm2, for holes and electrons, respectively [14]. Inthis case, Eq. 2.71b would be more appropriate than 2.71a for calculating thegeneration lifetime. In both cases, the generation lifetime is inversely proportionalto the number of generation centres, and, as would be expected, the leakage currentis proportional to this density.

However, if the only deep level centres are off mid-gap by more than a few kT,then, for those in the upper half of the band gap, en ep (and en ep if they arein the lower half). Taking, for example, a centre in the upper half of the band-gap,Eq. 2.66 reduces to:

JR qWNT ep 2:72

and the leakage current is limited by just the smaller of the two emission rateconstants (in this case ep), because, once the hole has been emitted, the followingstep of electron emission is so much faster that it has a negligible impact upon theoverall two stage emission process. Expanding ep:

JR qWNTrpvthni expET Ei=kT 2:73

) sg 1=NTrpvth expET Ei=kT 1=NTeff rpvth 2:74

NTeff NTexp ET Ei =kT, and is the equivalent number of mid-gapcentres, which would give the same leakage current. Hence, the shift in position ofa generation centre from mid-gap increases the generation lifetime by exp(ET-Ei)/kT, and decreases the leakage current by the same amount.

In summary, the reverse bias pn junction leakage current is characterised bythe generation lifetime, sg, which is related to the physical characteristics of thedeep level generation centres themselves.

34 2 Semiconductor Device Physics for TFTs

The other contribution to junction leakage current is the flow of minoritycarriers, into the reverse biased space region, from the adjacent neutral material. Inan n+p junction, this will be electrons from the p-type substrate, and those adjacentto the space charge region will be swept through it, and into the n+-region. Thisleaves a deficit of electrons at the depletion region edge, which establishes a localminority carrier concentration profile, thereby, driving a diffusion current, Jdiffn. Asthe ohmic contact to the p-type substrate cannot readily supply electrons, they needto be generated within the material by thermal generation, and the diffusion currentis determined by the generation lifetime, and is given by [4]:

Jdiffn qnpffiffiffiffiffiffiffiffiffiffiffiffiDn=sg

q2:75

Where np is the equilibrium electron concentration in the p-type substrate(=p0/ni

2), and Dn is the electron diffusion coefficient (=kTln/q). A significant dif-ference between the diffusion current and the generation current (Eq. 2.70) is thatthe diffusion current is not a function of the reverse bias voltage.

The treatment in this section has been limited to basic thermal emission pro-cesses, and these are directly used in the discussion of TFT leakage currents inSect. 8.4. In Sect. 8.5.3, the treatment is extended to include field-enhancedemission processes.

2.3.4 Recombination Processes

Recombination will occur in response to a steady state carrier injection process(such as above band-gap optical illumination), where the injection results in anincrease of the free carrier concentration above the thermal equilibrium values.The steady state carrier concentrations are given by the equality:

Rinj RR 2:76

Where Rinj is the injection rate, and RR is the recombination rate given byEq. 2.60 (or the equivalent Eqs. 2.61 and 2.62). As with the generation process, itis useful to simplify these equations to more physically meaningful forms. Forcharge neutrality, the injection process will result in an equality of the change intrap occupancy, and in the steady state excess densities of both holes and electrons,given by Dp and Dn, respectively. Where p = p0 ? Dp, and n = n0 ? Dn, and p0and n0 are the thermal equilibrium carrier densities, and n0p0 = ni

2.As with the discussion in the preceding sections, an n-type substrate is assumed,

and, depending upon the relative values of Dp and n0, two different injectionconditions are identified. When Dp n0, this is regarded as low-level injection,and when Dp C n0 this is defined as high-level injection.

2.3 Electron-Hole Pair Generation and Recombination 35

http://dx.doi.org/10.1007/978-3-319-00002-2_8http://dx.doi.org/10.1007/978-3-319-00002-2_8

2.3.4.1 Low-Level Injection

Consider an n-type substrate, with low-level injection, meaning that Dp n0, sothat n * n0. The low-level recombination lifetime, sR, is defined by:

RR Dp=sR 2:77

An examination of the physical recombination process will illustrate howEq. 2.60 can be simplified to yield a more tractable expression for the recombi-nation lifetime. Under low-level injection, the change in the free electron con-centration is so small that the equilibrium Fermi level can still be used to describethe electron concentration. Hence, all trap levels beneath the Fermi level are filledwith electrons, and ready to trap a hole as the first stage in the two-stagerecombination process. Having captured a hole, with the rate constantcp(p0 ? Dp), the subsequent electron capture will proceed with the rate constantcnn0, which, given that n0 (p0 ? Dp), will be a much faster process, and willnot rate limit the overall recombination process. The only other consideration iswhether the hole could be thermally emitted back into the valence band before theelectron capture process has been completed. For the electron capture rate toexceed the hole emission rate, we need cnn0 [ ep, i.e.:

cnNC expEC EF=kT [ cpNV expET=kT 2:78

i:e: ET [ EC EF kT lncpNV=cnNC 2:79

Taking the logarithmic term in Eq. 2.79 to be smaller than EC-EF, Eq. 2.79simply shows that, for efficient electron capture, the trap level must be further fromthe valence band edge than the Fermi level is from the conduction band edge. Inother words, providing the trap level, ET, is positioned somewhere between theFermi level and an equivalent distance from the valence band edge, the recom-bination process will be limited just by hole capture. Replacing n and p inEq. 2.62:

RR rnrpv2th NT n0Dp

cnn0 en cpp0 Dp ep2:80

From the above discussion, for EF [ ET [ EC-EF, then cnno [ en, ep, andcp(p0 ? Dp), and Eq. 2.80 reduces to:

RR rpvthNTDp Dp=sR 2:81

and sR 1=rpvthNT 2:82

In other words, the recombination lifetime is a function of the trap state density,NT, and the hole capture cross-section, and is independent of the trap energy levelover a substantial fraction of the band gap (as defined above). Equation 2.82 issimilar to the generation lifetime for a mid-gap generation centre (Eq. 2.71), but,in contrast to the recombination lifetime, once ET is more than a few kT from mid-

36 2 Semiconductor Device Physics for TFTs

gap, the generation lifetime increases substantially (as shown by Eq. 2.74).Therefore, except in the special case of a mid-gap centre, the steady state gener-ation and recombination lifetimes can be substantially different.

When ET lies outside the range prescribed for Eq. 2.81, the recombinationlifetime will increase. If ET [ EF, then the traps will be largely empty of electrons,and the number of traps available for hole capture will be low. In this situation,en [ cnn0, and Eq. 2.80 becomes:

RR rnrpv2thNT n0Dp

en rpvthNTDp expEF ET=kT 2:83

and sR expfET EF=kTg=rpvthNT for ET [ EF 2:84

Hence, as ET rises above EF, the lifetime is larger than that given by Eq. 2.82,and it increases exponentially with increasing values of ET.

Similarly, if the separation of ET from the valence band edge is smaller than thevalue of (EC - EF), then ep will exceed cnn0, and, from Eq. 2.80, the recombi-nation lifetime will be:

sR NV expEC EF ET=kT

NCrnvthNTfor ET EC EF 2:85

In other words, as the trap level gets closer to the valence band edge, and ETreduces, the lifetime exponentially increases, but is now controlled by the capturecross section for electrons, rather than for holes, as it has been in the previouscases.

2.3.4.2 High-Level Injection

As with low-level injection, the recombination process is described by the generalEq. 2.60 (or its equivalents), and to reduce these to a simpler form, the high-levelinjection situation of Dp n0 is considered. In this case, if Dp NT, then chargeneutrality will be determined just by equality in the excess free carrier densities,i.e. n = p = Dp = Dn, and the equilibrium Fermi level splits into separate quasi-Fermi levels, EFp and EFn, for holes and electrons, respectively, where the quasi-Fermi levels are given by:

p NVexp EFp=kT and n NCexp EC EFn =kT 2:86

If the recombination centre is sited between the quasi-Fermi levels, such thatEFp \ ET \ EFn, then ncn [ en and pcp [ ep, and the steady state recombinationcentre occupancy can be obtained from Eq. 2.58:

N0T NTrp

rn rp NT1 FD 2:87

2.3 Electron-Hole Pair Generation and Recombination 37

FD is the centres Fermi-Dirac function, given by Eq. 2.46, in which theequilibrium Fermi level, EF, is replaced by the quasi-Fermi level for the recom-bination centre, EFT. For the special case of equal capture cross sections, FD = 0.5,and the quasi-Fermi level for the recombination centre is located at ET.

For the recombination centre located between the hole and electron quasi-Fermilevels, the recombination lifetime, sR, can be calculated from Eqs. 2.60 and 2.77:

RR NTenep npcncpncn pcp en ep

NTDp2cncp

Dpcn Dpcp Dp

sR2:88

and

sR 1=rpvthNT 1=rnvthNT 2:89

Hence, the difference between the low-injection and high-injection lifetimes isthat, at high-injection, the lifetime explicitly accounts for the two-stage electronand hole capture process, and the lifetime is correspondingly longer. This is due tothe equal densities of holes and electrons. In contrast, the low-injection lifetimewas determined just by hole capture, due to the more rapid electron captureprocess resulting from the much higher majority carrier density of electrons.6

As with low-level injection, once the recombination level is outside the energyinterval bracketed by the carrier quasi-Fermi levels, the lifetime will increaseexponentially with this separation.

2.4 Current Flow Equations

The purpose of this section is to introduce the concepts underlying the modellingof current flow in semiconductor devices, so that the reader has an appreciation ofthe equations used in device simulation packages. As explained in the introduction,the numerical techniques used to solve these equations are beyond the scope of thisbook, and further information on device simulation can be found in Refs. [2] and[3].

To establish the basic equations, one-dimensional flow will be consideredinitially, and then extended to show the form used in 2-D or 3-D simulationprogrammes.

For current flow by carrier drift and diffusion, the total current density, JT, isgiven by the sum of the electron, Jn, and hole, Jp, drift/diffusion currents [1]:

JT Jn Jp 2:90

6 The situation described in Sects. 2.3.4.1 and 2.3.4.2 is for n-type substrates, and, for injectioninto p-type substrates, the low-level lifetime will be determined by electron capture.

38 2 Semiconductor Device Physics for TFTs

Jn qlnnF qDnon

ox2:91

Jp qlppF qDpop

ox2:92

Where F is the field, l is the carrier mobility, n and p are the free carrierdensities, and D is the diffusion coefficient. These are essentially low field equa-tions, because, as discussed below, at high fields, carrier velocity saturation canoccur [15], requiring the lF product to be replaced by the appropriate high fieldvelocity. In Eqs. 2.91 and 2.92, the first term describes the flow of carriers underthe influence of an internal field, which would result from an externally appliedbias, and the second term is the carrier flow by diffusion resulting from a non-uniform carrier distribution.

The continuity equation links these equations to local generation and recom-bination processes by:

on

ot Gn RGR

oJnqox

2:93

op

ot Gp RGR

oJpqox

2:94

These equations show that the local rate of change of carrier concentration,within a given volume of material, is determined by the difference in the externalcarrier generation rate, G, and the internal recombination rate, RGR, plus thedifference in the carrier flow into and out of the volume. In steady state, the localcarrier concentrations are constant, and Eqs. 2.93 and 2.94 are equal to zero. Theinternal recombination/generation rate, RGR, is given by Eq. 2.60 from Sect. 2.3.2,and the external generation rate, G, could be due to optical absorption of aboveband-gap light. In this case, the local optical generation rate, GO is:

Goz aU1 R expaz 2:95

Where a is the optical absorption coefficient, U is the incident photon flux, R isthe surface reflectivity, and z is the distance in the material perpendicular to theilluminated surface.7

Another potential source of carrier generation is high-field generation ofelectron-hole pairs by impact ionisation. This is also referred to as avalanchegeneration, since the generated carriers will also be accelerated by the field, andproduce further carriers by impact ionisation themselves. This is most likely tooccur with high carrier mobility semiconductors, and in high field regions ofdevices, such as reverse biased junctions. Where the carrier mobility is low, due toshort mean free paths and efficient scattering, the carrier is unlikely to gain enoughenergy from the field. However, where the mean free path is large, the carriers can

7 For a 1-D treatment, we require a\ z for uniform carrier generation.

2.4 Current Flow Equations 39

be efficiently accelerated and heated by the field. If the carriers attain sufficientenergy, then lattice collisions can lead to electron-hole pair generation. The impactionisation generation rate, GII, is given by [1]:

GII nvnan pvpap 2:96

Where vn (vp) is the electron (hole) drift velocity, an (ap) is the electron (hole)ionisation coefficient, and:

an;p qF

EIexpFC

F2:97

FC is the critical field, F is the field parallel to current flow, and EI is the carrierionisation energy (for Si this is 3.6 eV for electrons and 5.0 eV for holes). Asimpler expression [16] has also been used in simulations of TFTs [17], where theionisation coefficient is:

an;p a1n;p expFCF

2:98

and a? is a constant, which is determined, together with FC, from simulation fits.The carrier velocity, in Eq. 2.96, at low fields, is given by l0F, where l0 is the

low field mobility. At high fields, velocity saturation occurs, and the followingrelationship between velocity and field was found to provide a good fit to theexperimental c-Si data shown in Fig. 2.15 [15]:

vn;p l0F

1 l0F=vSbh i1=b 2:99

Where vS is the saturated velocity (*107 cm/s for holes and electrons in Si),

and b is a constant (*2 for electrons and *1 for holes in Si).

107

106

103 104 105 106

Electric Field (V/cm)

Car

rier V

eloc

ity (

cm/s

ec)

electrons

holes

I I I I IIIII I

Fig. 2.15 Carrier velocity measurements as a function of the electric field in silicon. The solidline is the empirical fit to Eq. 2.99 (Reprinted from [15] with permission of IEEE)

40 2 Semiconductor Device Physics for TFTs

Equations 2.902.94 contain the electrostatic field, F, which is the local gra-dient of the potential, dV/dx, and this has to be established in a self-consistentfashion by the simultaneous solution of Poissons equation:

d2V

dx2 qqx

e0es2:100

and q p n Nd Na NTd NTa 2:101

where Nd and Na are shallow donor and acceptor dopants, and NTa and NTd aredeep acceptor and donor defects, respectively. For a TFT, the deep levels couldequally well refer to a distribution of defect levels across the band-gap.

The above equations have been presented, for simplicity, in a 1-D format, but,for accurate device simulation, these equations need to be solved in two or threedimensions. In that case, the coupled equations in steady state are [18]:

r:rV qq=e0esr:Jn qGn RGRr:Jp qGp RGR

Jn qnlnrV qDnrnJp qplprV qDprp

2:102

These are solved subject to a set of boundary conditions determined by thebiases applied to the device terminals, the field continuity conditions acrossinternal material boundaries (such as the semiconductor/dielectric interface), andthe conditions at the external boundaries of the device, where, for instance, thefield may be clamped at zero.

In the commercial simulators used for Si-based TFTs, the internal recombi-nation/generation rate, RGR, includes additional processes to those considered inSect. 2.3. In particular, the treatment of carrier emission is extended to includefield-enhanced emission processes from traps, as well as band-to-band tunnelling.Those mechanisms are discussed further in Sect. 8.5.3.

2.5 Summary

Some analytical device physics concepts, using single crystal equations, have beenintroduced as a background topic to later chapters. These simple concepts arewidely used in interpreting TFT behaviour, and they provide a solid basis forappreciating the assumptions and approximations used in that work.

The topics in this chapter have been restricted to those of most relevance toTFTs, and have focussed, firstly, on aspects of semiconductor surface physics,

2.4 Current Flow Equations 41

http://dx.doi.org/10.1007/978-3-319-00002-2_8

which describe the relationship between gate bias, surface space charge, and bandbending in MIS structures. This topic underpins the understanding of IGFETbehaviour, which will be the subject of Chap. 3. The second topic is electron-holepair recombination and generation processes through deep level centres in theforbidden band gap. These processes play a role in establishing steady-state carrierconcentrations under injection processes, and determine reverse bias leakagecurrents from junction depletion regions. Finally, there is a brief overview of thecurrent flow processes, which are incorporated in device simulation packages.

Appendix: Summary of Key Equations

A number of the simplified equations from the text, which can be used in basicanalytical calculations, are reproduced below. The equation numbers are retainedfor quick reference back to the original derivations.

A.1 Semiconductor Surface Band Bending

Relationships between surface potential, Vs, space charge density, Qs, gate volt-age, VG, and threshold voltage, VT.

(a) Depletion and Inversion Space Charge Density

Qs ffi ffiffiffiffiffiffiffiffiffiffiffiffi2qe0es

pni

kT

qexp

qVs VFkT

NaVs 0:5

2:12

(b) Depletion Space Charge Density

Qs ffi ffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffi2qe0esNaVs

p2:13

(c) Gate Voltage, Surface Potential and Space Charge Density

VG Vs Qs=Ci 2:22

(d) Gate Threshold Voltage

VT VFB ffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffi2qe0esNa2VFp

Ci 2VF 2:28

and, from Eq. 2.5, VF = (kT/q)ln(Na/ni)

42 2 Semiconductor Device Physics for TFTs

http://dx.doi.org/10.1007/978-3-319-00002-2_3

(e) Depletion Layer Thickness at Inversion

xdmax ffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffi2e0es2VF

qNa

s2:18

(f) Flat-Band Voltage

VFB UMS Qieff=Ci Qss=Ci

A.2 Carrier Recombination and Generation

Relationships between trap density, NT, and capture cross section, r, and thecarrier generation/recombination rates.

(a) General Recombination and Generation Rate Expression

RGR rvthNT n2i np

n p 2nicoshET EikT2:63

(b) Generation Leakage Current

JR qniW=sg 2:70

(c) Generation Lifetime, sg

sg 1=0:5NTrvth 2:71a

(d) Carrier Recombination Rate, and Recombination Lifetime, sR

RR rpvthNTDp Dp=sR 2:81

(e) Recombination Lifetime (Low Injection Level)

sR 1=rpvthNT 2:82

(f) Recombination Lifetime (High Injection Level)

sR 1=rpvthNT 1=rnvthNT 2:89

2.5 Summary 43

References

1. Sze SM, Ng KK (2007) Physics of semiconductor devices, 3rd edn. Wiley, New York2. http://www.iue.tuwien.ac.at/phd/klima/node8.html (Accessed Aug 2010)3. http://www.silvaco.com/products/vwf/atlas/2D/tft/tft_03.pdf (Accessed Aug 2010)4. Grove AS (1967) Physics and technology of semiconductor devices. Wiley, New York,

pp 2782855. Deal BE, Snow EH, Mead CA (1966) Barrier energies in metalsilicon dioxidesilicon

structures. J Phys Chem Solids 27(1112):187318796. Brotherton SD, Gill A (1978) Determination of surface and bulk generation currents in low

leakage silicon MOS structures. Appl Phys Letts 33:8908927. Berglund CN (1966) Surface states at steam-grown siliconsilicon dioxide interface. IEEE

Trans Electron Dev 13(10):7017058. Castagne R, Vapaille A (1971) Description of the Si02Si interface properties by means of

very low frequency MOS capacitance measurements. Surf Sci 28(1):1571939. Nicollian EH, Goetzberger A (1967) The SiSiO2 interfaceelectrical properties as

determined by the MIS conductance technique. Bell Syst Tech J 46:105510. Hall RN (1952) Electron-hole recombination in germanium. Phys Rev 87(2):38711. Shockley W, Read WT (1952) Statistics of the recombination of holes and electrons. Phys

Rev 87(5):83584212. Sah CT, Noyce RN, Shockley W (1957) Carrier generation and recombination in pn

junction and pn junction characteristics. Proc IRE 45(9):1228124313. Lax M (1960) Cascade capture of electrons in solids. Phys Rev 119(5):1502152314. Brotherton SD, Bradley P (1982) Measurement of minority carrier capture cross sections and

application to gold and platinum in silicon. J Appl Phys 53(3):1543155315. Caughey DM, Thomas RE (1967) Carrier mobilities in silicon empirically related to doping

and field. Proc IEEE 55:2192219316. Chynoweth AG (1958) Ionisation rates for holes and electrons in silicon. Phys Rev

109(5):1537154017. Valletta A, Gaucci P, Mariucci L, Pecora A, Cuscun M, Maiolo L, Fortunato G (2010)

Threshold voltage in short channel polycrystalline silicon thin film transistors: Influence ofdrain induced barrier lowering and floating body effects. J Appl Phys 107:074505-1074505-9

18. Guerrieri G, Ciampolini P, Gnudi A, Rudan M, Baccarani G (1986) Numerical simulation ofpolycrystalline-silicon MOSFETs. IEEE Trans ED-33(8):12011206

44 2 Semiconductor Device Physics for TFTs

http://www.iue.tuwien.ac.at/phd/klima/node8.htmlhttp://www.silvaco.com/products/vwf/atlas/2D/tft/tft_03.pdf

http://www.springer.com/978-3-319-00001-5

2 Semiconductor Device Physics for TFTsAbstract2.1Introduction2.2Semiconductor Surface Physics2.2.1 Ideal MIS Capacitor and Surface Band Bending2.2.2 Gate Bias and Threshold VoltageThreshold Voltage2.2.3 Real MIS Structures2.2.3.1Work Function Differences2.2.3.2Oxide ChargesOxide Charges and Interface States

2.2.4 Evaluation of Surface Potential

2.3Electron-Hole Pair Generation and Recombination2.3.1 Thermal Equilibrium2.3.2 Non-equilibrium, Steady State2.3.3 Generation Currents2.3.4 Recombination Processes2.3.4.1Low-Level Injection2.3.4.2High-Level Injection

2.4Current Flow Equations2.5SummaryA.0. Appendix: Summary of Key EquationsA.0.0 A.1Semiconductor Surface Band BendingA.0.0 A.2Carrier Recombination and Generation

References